# A Novel Z Profile of Pultruded Glass-Fibre-Reinforced Polymer Beams for Purlins

^{1}

^{2}

^{*}

## Abstract

**:**

## 1. Introduction

## 2. Materials and Methods

#### 2.1. Optimum Profile of the Purlin

^{2}”. The live load was approximated to be “958 N/m

^{2}”, the rain load was “196 N/m

^{2}”, and the wind load was “993 N/m

^{2}”. Furthermore, the distance between two purlins was estimated to be 1.6 metres. Table 1 shows the intended loads on the purlin structure.

_{P}+ Q

_{S}+ Q

_{L}or Q = Q

_{P}+ Q

_{S}+ Q

_{R}+ Q

_{W}; where is the biggest

_{allowable}= 1/180

^{2}), C is the farthest point at the cross-section of the purlin and the neutral axis or z-z axis (m), I

_{z-z}is the moment of inertia of the cross-section of the purlin and the neutral axis (m

^{4}), V is the shear force at both fixed ends of the structure (N), Q is the area moment of the z-z axis (Nm), Â is the cross-section area above or below z-z axis (m

^{2}), ŷ is the centre gravity of the cross-section area above or below z-z axis from the z-z axis (m), δ is the deflection (m), and E is the modulus of elasticity of the pultruded GFRP material in the longitudinal direction (N/m

^{2}).

_{max}were “2037 N/m” and “13,750 Nm”, respectively.

_{t}), modulus of elasticity (E), and shear strength at the longitudinal axis (τ

_{L}) were “400 MPa”, “22 GPa”, and “40 MPa”, respectively [35]. As depicted in Figure 2, the purlin structure will produce one principal stress in the direction of the longitudinal axis of the purlin (x-x axis) and a deflection in the direction of the axis perpendicular to the longitudinal axis of the purlin (y-y axis). The stress and the deflection must be limited for the structure to be declared safe. Pultruded GFRP materials are brittle materials and do not have yield strength like steel. Therefore, the design stress (σ

_{d}) used as a safety limit in the FE approach analysis was 80% of the tensile strength or “320 MPa”. Then, the analysis used a theoretical-analytic approach using allowable stress by taking a safety factor of 3, because this considers the stress concentration due to the bolt holes [36] at the supports at both ends of the purlin. Thus, the allowable stress (σ

_{allowable}) was “106.67 MPa”. The flexural stress was calculated using Equation (3). As described above, the failure of flexural stress mode occurs at both ends of the supports. On the other hand, the failure of the shear mode is caused by shear forces at both ends of the purlin structure. The most significant shear stress will occur at the line of the neutral axis (z-z axis) and at the plane where the longitudinal axis (x-x axis) is present. Equation (4) is the formula for calculating shear stress. Maximum deflection occurs in the middle of the span of the purlin structure and is calculated by Equation (5). Referring to Table 9.5.b of ACI 318-19 [37], the magnitude of the deflection was limited to L/180, as shown in Equation (6).

#### 2.2. Purlin Prototypes and Structures

^{2}” stitched mat of Jushi EMK450 (Changzhou Zhongjie Composites Co., Ltd., Changzhou, China). Meanwhile, the polymer matrix was a mixture of 100 parts by weight of orthophthalic unsaturated polyester resin (UPR) SHCP 3316QN (PT SHCP Indonesia, Surabaya, Indonesia), five elements by weight of alumina trihydrate (ATH) H-WF-08A (PT Justus Kimiaraya, Jakarta, Indonesia), five parts by weight of light-grey pigments HM IP 7 (PT Mata Pelangi Chemindo, Jakarta, Indonesia), and one and a half parts by weight of catalyst benzoyl peroxide BENZOXE-N (PT Kawaguchi Kimia Indonesia, Jakarta, Indonesia). Fibre and matrix weight percentages in the composite were 55–60% and 45–40%, respectively [35]. All these materials were procured from PT Intec Persada, Indonesia.

#### 2.3. Finite Element Analysis of the Purlin Structure

## 3. Results

#### 3.1. Purlin Profile

_{z-z})

_{min}, was calculated as “31.640 × 10

^{−6}m

^{4}”or “31.640 × 10

^{6}mm

^{4}”.

_{max}= (13,750 × 0.125)/(31.976 × 10

^{−6}) = “53.75 MPa” < σ

_{allowable}= “106.67 MPa” → OK

_{max}= (2037 × 9

^{4})/(384 × 22 × 10

^{9}× 31.976 × 10

^{−6}) = “0.0495 m” = “49.5 mm”

_{max}= 0.0495/9 = 1/181 < (δ/L)

_{allowable}= 1/180 → OK

#### 3.2. Purlin Prototypes and Structure

_{55–45}) and another purlin with ratio 60–40% (Z

_{60–40}). Barcol hardness examination on several points of the two samples’ surfaces yielded relatively similar results in the 55–60 range. Tensile tests were conducted following the ASTM D638 standard for the two samples in the longitudinal and transverse directions. Likewise, the shear strength test in the direction of the longitudinal axis of the bar was carried out according to the procedure described in Figure 3. Table 5 shows both samples’ longitudinal and transverse tensile properties and longitudinal shear strength.

#### 3.3. Finite Element Model of the Purlin Structure

^{2}; 0.34; 1000 N/mm

^{2}; 1940 kg/m

^{3}; 320 N/mm

^{2}; 0.15 W/mK; and 1400 J/kg K, respectively. The external force was loaded as a uniformly distributed force along the purlin, Q. Initially, we used the data properties in Table 2 as parameters input in the FE model of Figure 5. The properties are modulus of elasticity, Poisson’s ratio, shear modulus, mass density, tensile strength, thermal conductivity, and specific heat. The value taken for these parameters are, respectively, 22,000 N/mm

^{2}; 0.32; 1000 N/mm

^{2}; 1900 kg/m

^{3}; 320 N/mm

^{2}; 0.15 W/m K; and 1400 J/kg K. We compared the deflection of the end of the cantilever structure with the deflection of the experimental results as a reference. Next, we changed some properties of the FE model to obtain a deflection value similar to the experimental reference value. Finally, the properties modulus of elasticity, Poisson’s ratio, and mass density were adjusted to be, respectively, 20,400 N/mm

^{2}; 0.34; and 1940 kg/m

^{3}.

## 4. Discussion

_{60–40}, with a 60–40 reinforcement–matrix weight ratio. The pultruded GFRP purlin cross-section has a height (h) of “250 mm”, a width (w) of “100 mm”, and a thickness (t) of “8 mm”. The moment of inertia along the neutral axis (I

_{z–z}) was “31.976 × 10

^{−6}m

^{4}”.

_{60–40}pultruded GFRP material in Table 5 indicate “433 ± 21.24 MPa” longitudinal tensile strength, “22,440 ± 218 MPa” modulus of elasticity, and “45.5 ± 2.4 MPa” longitudinal shear strength.

_{60–40}pultruded GFRP beam was the optimum design for the nine-metre-span purlin to suit a new warehouse building in the fertiliser industry.

_{55–45}and Z

_{60–40}have reinforcement–matrix weight ratios of 55–60% and 45–40%, respectively, while the volume ratios are 41–47% and 59–53%.

_{60–40}, has yielded good results: the tensile properties were observed under the design requirements. When making pultruded composites, some researchers may use fibre with volume fractions from 40–80%, depending on the production methods [50,51]. The greater the amount of reinforcement, the higher the strength and stiffness of the resulting composite. E-glass longitudinal fibres provide the necessary strength and stiffness. Four E-glass stitched mats were included to provide adequate strength and rigidity in the transverse direction.

_{60–40}, the tensile strength in the transverse direction, as denoted in Table 5, was “70 ± 8.15 MPa”. The trial production verified the success of the design and production of the Z prototype purlins, which met the technical criteria. Furthermore, purlin assembly with bolt-nut connections and sag-rod stiffening, as shown in Figure 11 and Figure 12, demonstrated that the purlin roof-support structure functions properly.

## 5. Conclusions

## 6. Patents

## Author Contributions

## Funding

## Institutional Review Board Statement

## Informed Consent Statement

## Data Availability Statement

## Acknowledgments

## Conflicts of Interest

## References

- Wojnar, A.; Sieńkowska, K. Comparison of strength and stiffness parameters of purlins with different cross-sections of profiles. Open Eng.
**2020**, 10, 604–611. [Google Scholar] [CrossRef] - Sun, M.; Packer, J.A. Hot-dip galvanizing of cold-formed steel hollow sections: A state-of-the-art review. Front. Struct. Civ. Eng.
**2019**, 13, 49–651. [Google Scholar] [CrossRef] - Ivan, S.C. Recent progress and required developments in atmospheric corrosion of galvanised steel and zinc. Materials
**2017**, 10, 1288. [Google Scholar] [CrossRef][Green Version] - Zhang, Z.; Xu, S.; Li, R. Comparative investigation of the effect of corrosion on the mechanical properties of different parts of thin-walled steel. Thin-Walled Struct.
**2020**, 146, 106450. [Google Scholar] [CrossRef] - Silva, R.S.; Meneguzzi, A. Passivation of carbon steel using intelligent epoxy paint. Coatings
**2020**, 10, 452. [Google Scholar] [CrossRef] - Tiano, P.C.M.; Aoki, I.V. Corrosion protection of steel structures in industrial and marine atmospheres by waterborne acrylics DTM (direct to metal) paint system. In Proceedings of the European Corrosion Congress, EUROCORR 2015, Austria, Graz, 6–10 September 2015; p. 128475. [Google Scholar]
- Qureshi, J. A Review of Fibre Reinforced Polymer Structures. Fibers
**2022**, 10, 27. [Google Scholar] [CrossRef] - Hollaway, L.C. A review of the present and future utilisation of FRP composites in the civil infrastructure with reference to their important in-service properties. Constr. Build. Mater.
**2019**, 24, 2419–2445. [Google Scholar] [CrossRef] - Vedernikov, A.; Safonov, A.; Tucci, F.; Carlone, P.; Akhatov, I. Pultruded materials and structures: A review. J. Compos. Mater.
**2020**, 54, 4081–4117. [Google Scholar] [CrossRef] - Shin, Y.H.; Yoong, Y.Y.; Hejazi, F.; Saifulnaz, M.R.R. Review on pultruded FRP structural design for building construction. In Proceedings of the IOP Conference Series: Earth and Environmental Science, Sustainable Civil and Construction Engineering Conference, Kuala Lumpur, Malaysia, 25–27 August 2018; Volume 357, p. 012006. [Google Scholar] [CrossRef]
- Correia, J.R.; Fonseca, S.C.; Branco, F.A.; Ferreira, J.; Eusébio, M.I.; Rodrigues, M.P. Durability of glass fiber reinforced polyester (GFRP) pultruded profiles for construction applications. Mech. Compos. Mater.
**2006**, 42, 325–338. [Google Scholar] [CrossRef] - Correia, J.R.; Branco, F.A.; Ferreira, J.; Fonseca, S.C.; Rodrigues, J.P.C. Lifetime performance of GFRP pultruded profiles for structural applications. In Proceedings of the IABSE Symposium Improving Infrastructure—Bringing People Closer Worldwide, Weimar, Germany, 19–21 September 2007. [Google Scholar] [CrossRef]
- Beura, S.; Thatoi, D.N.; Chakraverty, A.P.; Mohanty, U.K. Impact of the ambiance on GFRP composites and role of some inherent factors: A review report. J. Reinf. Plast. Compos.
**2018**, 37, 533–547. [Google Scholar] [CrossRef] - Grmmatikos, S.A.; Jones, R.G.; Evernden, M.; Correia, J.R. Thermal cycling effects on the durability of a pultruded GFRP material for off-shore civil engineering structures. Compos. Struct.
**2016**, 153, 297–310. [Google Scholar] [CrossRef][Green Version] - Zhang, L.; Liu, W.; Wang, L.; Ling, Z. On-axis and off-axis compressive behavior of pultruded GFRP composites at elevated temperatures. Compos. Struct.
**2020**, 236, 111891. [Google Scholar] [CrossRef] - Jafari, A.; Ashafi, H.; Bazli, M.; Ozbakkaloglu, T. Effect of thermal cycles on mechanical response of pultruded glass fiber reinforced polymer profiles of different geometries. Compos. Struct.
**2019**, 223, 110959. [Google Scholar] [CrossRef] - Bazli, M.; Jafari, A.; Ashrafi, H.; Zhao, X.L.; Bai, Y.; Singh-Raman, R.K. Effects of UV radiation, moisture and elevated temperature on mechanical properties of GFRP pultruded profiles. Constr. Build. Mater.
**2020**, 231, 117137. [Google Scholar] [CrossRef] - Setyanto, D. The possibility of E-glass woven roving as reinforcement of GFRP composite sheet roof. AIP Conf. Proc.
**2016**, 1717, 040007. [Google Scholar] [CrossRef] - Fitzgerald, A.M.; Wong, N.; Fitzgerald, A.V.L.; Jesson, D.A.; Martin, F.; Murphy, R.J.; Young, T.; Hamerton, I.; Longana, M.L. Life Cycle Assessment of the High Performance Discontinuous Fibre (HiPerDiF) Technology and Its Operation in Various Countries. Sustainability
**2022**, 14, 1922. [Google Scholar] [CrossRef] - Joustra, J.; Flipsen, B.; Balkenende, R. Circular Design of Composite Products: A Framework Based on Insights from Literature and Industry. Sustainability
**2021**, 13, 7223. [Google Scholar] [CrossRef] - Fitzgerald, A.; Proud, W.; Kandemir, A.; Murphy, R.J.; Jesson, D.A.; Trask, R.S.; Hamerton, I.; Longana, M.L. A Life Cycle Engineering Perspective on Biocomposites as a Solution for a Sustainable Recovery. Sustainability
**2021**, 13, 1160. [Google Scholar] [CrossRef] - Chard, J.M.; Basson, L.; Creech, G.; Jesson, D.A.; Smith, P.A. Shades of Green: Life Cycle Assessment of a Urethane Methacrylate/Unsaturated Polyester Resin System for Composite Materials. Sustainability
**2019**, 11, 1001. [Google Scholar] [CrossRef][Green Version] - Ribeiro, M.C.S.; Fiúza, A.; Ferreira, A.; Dinis, M.D.L.; Castro, A.C.M.; Meixedo, J.P.M.; Alvim, M.R. Recycling Approach towards Sustainability Advance of Composite Materials’ Industry. Recycling
**2016**, 1, 178–193. [Google Scholar] [CrossRef][Green Version] - Krauklis, A.E.; Karl, C.W.; Gagani, A.I.; Jørgensen, J.K. Composite Material Recycling Technology—State-of-the-Art and Sustainable Development for the 2020s. J. Compos. Sci.
**2021**, 5, 28. [Google Scholar] [CrossRef] - Nurazzi, N.M.; Asyraf, M.R.M.; Khalina, A.; Abdullah, N.; Aisyah, H.A.; Rafiqah, S.A.; Sabaruddin, F.A.; Kamarudin, S.H.; Norrrahim, M.N.F.; Ilyas, R.A.; et al. A Review on Natural Fiber Reinforced Polymer Composite for Bullet Proof and Ballistic Applications. Polymers
**2021**, 13, 646. [Google Scholar] [CrossRef] [PubMed] - Muc, A.; Stawiarski, A.; Chwal, M. Design of the hybrid FRP/concrete structures for bridge constructions. Compos. Struct.
**2020**, 2471, 112490. [Google Scholar] [CrossRef] - Salakhutdinov, M.A.; Gimranov, L.R.; Kuznetsov, I.L.; Fakhrutdinov, A.E.; Nurgaleeva, L.M. PFRP structures under the predominately short-term load. Mag. Civ. Eng.
**2020**, 96, 3–14. Available online: https://engstroy.spbstu.ru/userfiles/files/2020/4(96)/01.pdf (accessed on 28 February 2022). [CrossRef] - Russo, S. On failure modes and design of multi-bolted FRP plate in structural joints. Compos. Struct.
**2019**, 218, 325–334. [Google Scholar] [CrossRef] - Cavaleri, L.; Di Paola, M.; Ferrotto, M.F.; Scalici, T.; Valenza, A. Structural performances of pultruded GFRP emergency structures—Part 1: Experimental characterization of materials and substructure. Compos. Struct.
**2019**, 214, 325–334. [Google Scholar] [CrossRef] - Cavaleri, L.; Di Paola, M.; Ferrotto, M.F.; Scalici, T.; Valenza, A. Structural performances of pultruded GFRP emergency structures—Part 2: Full-scale experimental testing. Compos. Struct.
**2019**, 214, 304–315. Available online: https://pure.unipa.it/en/publications/structural-performances-of-pultruded-gfrp-emergency-structures-pa (accessed on 28 February 2022). [CrossRef] - Hou, J.; Nie, X.; Zhang, L.; Huang, Y.; Bai, Y. Ultimate limit design of composite beams with modular GFRP deck and steel girder. Eng. Struct.
**2018**, 176, 337–348. [Google Scholar] [CrossRef] - Yang, X.; Bai, Y.; Luo, F.J.; Zhao, X.L.; Ding, F. Dynamic and fatigue performances of a large-scale space frame assembled using pultruded GFRP composites. Compos. Struct.
**2016**, 138, 227–236. [Google Scholar] [CrossRef] - Pahl, G.; Beitz, W.; Feldhusen, J.; Grote, K.H. Engineering Design—A Systematic Approach, 3rd ed.; Springer: London, UK, 2007; pp. 63–124. [Google Scholar]
- Indonesian National Standard SNI 1727. 2000. Available online: http://sispk.bsn.go.id/sni/DetailSNI/12927 (accessed on 28 February 2022).
- Xin, H.; Liu, Y.; Mosallam, A.S.; He, J.; Du, A. Evaluation on material behaviors of pultruded glass fiber reinforced polymer (GFRP) laminates. Compos. Struct.
**2017**, 182, 283–300. [Google Scholar] [CrossRef][Green Version] - Zhuang, L.; Su, B.; Lin, M.; Liao, Y.; Peng, Y.; Zhou, Y.; Luo, D. Influence of the property of hole on stress concentration factor for isotropic plates. In Proceedings of the 10th International Conference on Composite Science and Technology, Instituto Superior Tecnico, Lisboa, Portugal, 2–4 September 2015; Available online: http://www.dem.ist.utl.pt/iccst10/files/ICCST10_Proceedings/pdf/WEB_PAPERS/ICCST10_Upload_153.pdf (accessed on 28 February 2022).
- ACI Committee 318. Building Code Requirements for Structural Concrete (ACI 318-19) an ACI Standard; American Concrete Institute: Farmington Hills, MI, USA, 2019; Available online: https://www.concrete.org/ (accessed on 28 February 2022).
- ASTM D2583 Standard. Available online: https://www.astm.org/d2583-13a.html (accessed on 28 February 2022).
- ASTM D638 Standard. Available online: https://www.astm.org/d0638-14.html (accessed on 28 February 2022).
- Li, C.; Xian, B. Mechanical property evolution and life prediction of carbon fiber and pultruded carbon fiber reinforced polymer plate exposed to elevated temperatures. Polym. Compos.
**2020**, 41, 5143–5155. [Google Scholar] [CrossRef] - Priyanka, P.; Dixit, A.; Mali, H.S. High strength Kevlar fiber reinforced advanced textile composites (Review). Iran. Polym. J.
**2019**, 28, 621–638. [Google Scholar] [CrossRef] - Alam, P.; Mamalis, D.; Robert, C.; Floreani, C.; Bradaigh, C.M.Ó. The fatigue of carbon fiber reinforced plastics—A review. Compos. Part B
**2019**, 166, 555–579. [Google Scholar] [CrossRef][Green Version] - Karatas, M.A.; Gokkaya, H. A review on machinability of carbon fiber reinforced polymer (CFRP) and glass fiber reinforced polymer (GFRP) composite materials. Def. Technol.
**2018**, 14, 318–326. [Google Scholar] [CrossRef] - Zhang, S.; Caprani, C.C.; Heidarpour, A. Strain rate studies of pultruded glass fiber reinforced polymer material properties: A literature review. Constr. Build. Mater.
**2018**, 171, 984–1004. [Google Scholar] [CrossRef] - Fernandes, L.A.; Silvestre, N.; Correia, J.R.; Arruda, M.R.T. Fracture toughness-based models for damage simulation of pultruded GFRP materials. Compos. Part B
**2020**, 186, 107818. [Google Scholar] [CrossRef] - Saykin, V.V.; Nguyen, T.H.; Hajjar, J.F.; Deniz, D.; Song, J. Validation of a finite element approach to modeling of structural collapse of steel structures. In Proceedings of the Structures Congress, Boston, MA, USA, 3–5 April 2014; pp. 2162–2173. [Google Scholar] [CrossRef][Green Version]
- Mantovani, D.P.; Rohen, L.A.; Neves, A.C.C.; Vieira, J.S.; Pontes, L.A.P.; Vieira, C.M.F.; Margem, F.M.; Monteiro, S.M. Comparative analysis of the tensile properties of polyester to epoxy matrixes composites reinforced with hemp fibers. In Proceedings of the 6th International workshop advances in cleaner production, Sao Paulo, Brasil, 24–26 May 2017; Available online: http://www.advancesincleanerproduction.net/sixth/files/sessoes/6B/5/mantovani_dp_et_al_academic.pdf (accessed on 28 February 2022).
- Ramadan, N.; Taha, M.; La Rosa, A.D.; Elsabbagh, A. Towards selection charts for epoxy resin, unsaturated polyester resin and their fibre fabric composites with flame retardants. Materials
**2021**, 14, 1181. [Google Scholar] [CrossRef] - Wu, W.; Wang, Q.; Li, W. Comparison of tensile and compressive properties of carbon/glass interlayer and intralayer hybrid composite. Materials
**2021**, 11, 1105. [Google Scholar] [CrossRef][Green Version] - Shakya, N.S.; Roux, J.A.; Jeswani, A.L. Effect of fiber volume fraction in fiber reinforcement compaction in resin injection pultrusion process. Polym. Polym. Compos.
**2016**, 24, 7–20. [Google Scholar] [CrossRef] - Hashemi, F.; Tahir, P.M.; Madsen, B.; Jawaid, M.; Majid, D.L.; Branscheriau, L.; Juliana, A.H. Volumetric composition and shear strength evaluation of pultruded hybrid kenaf/glass fiber composites. J. Compos. Mater.
**2016**, 15, 2291–2303. [Google Scholar] [CrossRef]

**Figure 13.**The correlation between force and deflection from experimental and FE models of the cantilever structure.

Technical Loads | Constant Distributed Forces |
---|---|

Purlin weight (“7.25 kg/m” or “71 N/m”) | Q_{P} = “71 N/m” |

GFRP roofing sheet weight (“4 kg/m^{2}” or “39 N/m^{2}”) | Q_{S} = “63 N/m” |

Live load (“20 psf” or “97.6 kg/m^{2}” or “958 N/m^{2}”) | Q_{L} = “1532 N/m” |

Rain load (“20 kg/m^{2}” or “196 N/m^{2}”) | Q_{R} = “314 N/m” |

Wind load (“90 mph” or “993 N/m^{2}”) | Q_{W} = “1589 N/m” |

**Table 2.**Minimum mechanical properties of the pultruded GFRP beam material in the longitudinal direction.

Properties | Value |
---|---|

Tensile strength, σ_{t} | “400 × 10^{6} N/m^{2}” |

Design tensile strength, σ_{d} | “320 × 10^{6} N/m^{2}” |

Modulus of elasticity, E | “22 × 10^{9} N/m^{2}” |

Longitudinal shear strength, τ_{L} | “40 × 10^{6} N/m^{2}” |

Poisson ratio, ν | 0.32 |

Sub-Functions | Alternative Solutions | |||
---|---|---|---|---|

1st Solution | 2nd Solution | 3rd Solution | 4th Solution | |

Withstands corrosive environment | GFRP | KFRP | CFRP | Hybrid of G/K/C-FRP |

Withstands all technical loads | Pultruded beam with continuous roving and stitched mat reinforcement | |||

Compact for handling and shipping | Z profile | C profile | Ω profile | - |

Moment of Inertia (×10^{6} mm^{4}) | Thickness t (mm) | Height h (mm) | Width w (mm) | Cross-Section area A (mm^{2}) | |
---|---|---|---|---|---|

(I_{z}_{-z})_{min} | (I_{z}_{-z})_{actual} | ||||

31.640 | 31.956 | 40 | 180 | 70 | 9912 |

31.640 | 32.251 | 21 | 200 | 75 | 6468 |

31.640 | 32.058 | 14 | 220 | 80 | 4928 |

31.640 | 32.693 | 10 | 240 | 90 | 4000 |

31.640 | 31.976 | 8 | 250 | 100 | 3472 |

Tensile Properties | Samples Material | |
---|---|---|

Z_{55–45} | Z_{60–40} | |

Longitudinal tensile strength | “396 ± 24.02 MPa” | “433 ± 21.24 MPa” |

Longitudinal modulus of elasticity | “21,104 ± 198 MPa” | “22,440 ± 218 MPa” |

Transversal tensile strength | “76 ± 7.23 MPa” | “70 ± 8.15 MPa” |

Transversal modulus of elasticity | “6586 ± 82 MPa” | “6230 ± 69 MPa” |

Longitudinal shear strength | “41.8 ± 2.1 MPa” | “45.5 ± 2.4 MPa” |

Loads (kg) | Deflection at the Free End | ||
---|---|---|---|

Experimental Model (mm) | FE Model (mm) | Difference | |

0 | 0 | 0 | 0% |

46.39 | 4.4 | 4.53 | −2.96% |

69.59 | 7.0 | 6.80 | −2.86% |

92.78 | 9,0 | 9.07 | 0.78% |

115.98 | 110 | 11.35 | 3.18% |

139.18 | 13.0 | 13.61 | 4.69% |

162.37 | 16.5 | 15.88 | −3.76% |

185.57 | 19.0 | 18.15 | −4.47% |

208.76 | 22.0 | 20.42 | −7.18% |

Publisher’s Note: MDPI stays neutral with regard to jurisdictional claims in published maps and institutional affiliations. |

© 2022 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (https://creativecommons.org/licenses/by/4.0/).

## Share and Cite

**MDPI and ACS Style**

Setyanto, D.; Antonio, Y.A.; Darmawan, M.; Ubaidillah, U.
A Novel Z Profile of Pultruded Glass-Fibre-Reinforced Polymer Beams for Purlins. *Sustainability* **2022**, *14*, 5862.
https://doi.org/10.3390/su14105862

**AMA Style**

Setyanto D, Antonio YA, Darmawan M, Ubaidillah U.
A Novel Z Profile of Pultruded Glass-Fibre-Reinforced Polymer Beams for Purlins. *Sustainability*. 2022; 14(10):5862.
https://doi.org/10.3390/su14105862

**Chicago/Turabian Style**

Setyanto, Djoko, Yohanes Adeatma Antonio, Marten Darmawan, and Ubaidillah Ubaidillah.
2022. "A Novel Z Profile of Pultruded Glass-Fibre-Reinforced Polymer Beams for Purlins" *Sustainability* 14, no. 10: 5862.
https://doi.org/10.3390/su14105862